Bimetallic core/shell nanoparticle-decorated 3D urchin-like hierarchical TiO2 nanostructures with magneto-responsive and decolorization characteristics
© Xiang et al.; licensee Springer. 2015
Received: 28 November 2014
Accepted: 9 February 2015
Published: 27 February 2015
The semiconductors decorated with noble metals or magnetic metals have attracted increasing attention due to multifunctional properties. In this article, we prepare novel bimetallic core/shell nanoparticle (Co@Au and Co@Ag)-decorated 3D urchin-like hierarchical TiO2 nanostructures through combining electroless plating and in situ replacement processes. The morphology and structure are characterized by scanning electron microscopy, transmission electron microscopy, energy-dispersive spectroscopy, and a surface area analyzer. It demonstrates that Co@Au and Co@Ag nanoparticles are uniformly decorated on urchin-like TiO2 nanostructures. The composite nanostructures show not only surface plasmon absorption band from Au or Ag but also a magneto-responsive characteristic from Co. This allows composite nanostructures to exhibit advantages including enhanced decolorization efficiency compared to pure TiO2 nanostructures and facile separation from a solution by magnetic field.
The combinations of semiconductors with noble metals or magnet metals have been demonstrated to be interesting in fields ranging from catalysis and optics to biotechnology . Besides doping noble metals or magnet metals into semiconductors, the assembly of noble metal or magnetic metal nanoparticles onto semiconductors with special morphology, such as nanospheres, tubes and wires, films, and even three-dimensional nanostructures, has raised great interest [2,3]. Different from doped systems, the composite nanostructures may combine the unique properties of semiconductors and noble metals or magnetic metals and show multifunctional behaviors [2,3].
Titania (TiO2) is a high-performance functional material with a wide range of applications due to its semiconductive and biocompatible natures . TiO2 decorated with nanoparticles of noble metal has attracted enormous attention. However, the simultaneous and effective control of the composition, morphology, structure, and distribution of decorated nanoparticles is still a challenge. In recent years, a lot of effort has been made on the study of TiO2 microspheres decorated with monometallic nanoparticles. And even there are a few reports about 3D hierarchical TiO2 microspheres decorated with noble metal nanoparticles. In the previous work, we have prepared a kind of Au or Ag nanoparticle-decorated 3D urchin-like TiO2 nanostructures, which exhibit an enhanced photocatalytic activity compared with the pure urchin-like TiO2 nanostructures and commercial P25 photocatalyst . However, the percentages of methyl blue degraded by Ag-decorated TiO2 and Au-decorated TiO2 are only about 78% and 68% after 3 h of UV–vis light irradiation . So, there is still a large space to improve on the degraded efficiency.
Bimetallic nanostructures often exhibit improved physical and chemical properties over their monometallic counterpart and hence are useful in many applications . Especially, core/shell nanoparticles with a magnetic core and a noble-metallic shell have attracted a great deal of attention . The magnetic core can provide magnetic functionality and delivery power and the noble-metallic shell can offer a well-developed function, such as surface for biomolecule attachment and plasmonically active components for optical imaging . Core/shell nanoparticles, such as Fe3O4/Au, Co/Ag, and Co@Au, have attracted considerable attention [9-11]. These materials have great potential applications in the areas of electronics, photonics, catalysis, biotechnology, and so on.
Herein, we report novel 3D hierarchical TiO2 nanostructures decorated with bimetallic nanoparticles that have a magnetic cobalt core and a silver or gold nanoshell. The samples are prepared through a two-step method involving electroless plating and in situ replacement processes. The resulting composite 3D nanostructures show a distinct surface plasmon absorption band in the visible region and a good magnetic response to an external magnetic field. Furthermore, the composite 3D nanostructures can quickly decolorize methyl blue solution at room temperature. The bimetallic nature and 3D hierarchical architecture have shown excellent properties in extensive application. The combination of such bimetallic nanoparticles and TiO2 with a hierarchical nanostructure can not only combine multiple functionalities of dissimilar materials but also address the aggregation of nanoparticles. To the best of our knowledge, there is no report of the synthesis of the magnetically bimetallic core-shell nanospheres-decorated 3D hierarchical TiO2 nanostructures. We present here the preparation, characterization, and the properties of two kinds of magnetically bimetallic core-shell nanoparticles (Co@Au and Co@Ag)-decorated 3D urchin-like hierarchical TiO2 nanostructures in detail.
Synthesis of hierarchical TiO2 nanostructures
Hierarchical TiO2 nanostructures were obtained by a solvothermal method described in our previous article [12,13]. In a typical synthesis, tributyltin chloride (TBT) was dissolved in toluene in an ice-water bath, and subsequently, TiCl4 aqueous solution was added dropwise into the TBT/toluene solution under stirring. The mixture was transferred into a stainless steel autoclave lined with Teflon and heated at 150°C for 24 h. The precipitates were filtered, washed with ethanol several times, and dried to obtain urchin-like 3D hierarchical TiO2 nanostructures.
Pre-activation of hierarchical TiO2 nanostructures
In order to decorate with metal nanoparticles, TiO2 nanostructures were pre-activated by the method as described in Ref. . Firstly, the TiO2 particles were dispersed in a solution of 0.1 M SnCl2/0.1 M HCl for 40 min. During this process, the ‘sensitizer’ (Sn2+) was modified onto the surface of TiO2 nanostructures. Then, the particles were washed with water and centrifuged, and the supernant was discarded. Subsequently, the Sn2+-sensitized TiO2 nanostructures were dispersed in an aqueous solution of 1.5 × 10−3 M PdCl2/0.25 M HCl for another 40 min. During this process, the ‘catalyzer’ (Pd crystal seeds) was deposited onto the surface of TiO2 nanostructures. Finally, the particles were washed with water again by centrifugation to get Pd-modified TiO2 nanostructures.
Synthesis of Co nanoparticle-decorated hierarchical TiO2 nanostructures
An amount of 0.5 g of activated TiO2 particles was dispersed in an aqueous CoCl2 solution (50 mL, 0.01 to 0.025 M) by mechanical stirring. Then, the suspension was protected by N2 and placed in a water bath at 30°C. After stirring for 1 h, a freshly prepared and ice-cold NaBH4 solution (80 mL, 0.005 to 0.015 M) was added dropwise with the rate of 2 mL/min. Within several minutes, the color of suspension changed from pink to dark gray, indicating the formation of Co nanoparticles. After further reaction for 40 min under stirring, the precipitate was separated by a magnet and washed with water three times to get Co nanoparticle-decorated TiO2 nanostructures. They are named as Co/TiO2.
Synthesis of Co@Au or Co@Ag nanoparticle-decorated hierarchical TiO2 nanostructures
Co@Au or Co@Ag nanoparticles are facilely prepared at room temperature by in situ replacement reaction, in which Co nanoparticles are partly replaced by a noble metal salt. The process is shown as follows: 0.2 g of Co nanoparticle-decorated TiO2 nanostructures were dispersed into an aqueous HAuCl4 solution (50 mL, 0.5× 10−3 M) or AgNO3 solution (50 mL, 1.5 × 10−3 M) by mechanical stirring. After stirring for 1 h, the precipitate was centrifuged and washed with water three times to get resulting Co@Au or Co@Ag nanoparticles-decorated hierarchical TiO2 nanostructures. They are named as Co@Au/TiO2 or Co@Ag/TiO2.
The morphology of samples was observed by scanning electron microscopy (SEM; JSM-6700 F, Electron Optics Laboratory Co., Ltd, Tokyo, Japan) and transmission electron microscopy (TEM; JEOL-3010, Electron Optics Laboratory Co., Ltd, Tokyo, Japan). The chemical composition of samples was analyzed by transmission electron microscopy equipped with energy-dispersive X-ray (TEM/EDX; JEOL-3010, Electron Optics Laboratory Co., Ltd, Tokyo, Japan) spectroscopy. The special surface areas were determined by a Quantachrome Nova2000e surface area and pore size analyzer (Quantachrome Instruments, Boynton Beach, FL, USA). Absorbance spectra were measured using UV–vis spectrophotometer (HITACHI U-4100, HITACHI High-Technologies Corporation, Tokyo, Japan).
Analytical-grade methyl blue (MB, molecular formula: C37H27N3Na2O9S3, supplier: Tianjin Chemical Reagent Co. Ltd of China) was served as the target dye. Decolorization experiments are conducted at room temperature with a prepared solution of 40 mg/L MB dye in a 100-mL beaker. Typically, 10 mg of pure urchin-like TiO2, Co@Au/TiO2 or Co@Ag/TiO2 were respectively added into 30 mL of MB aqueous solution. After the suspension was stirred for about 15 min under daylight lamp of 40 W, the catalyst was separated by centrifugation and the reaction mixture was analyzed by UV–vis spectrophotometer (HITACHI U-4100).
Results and discussion
Figure 3 shows the typical morphology, structure, and composition of the Co@Au/TiO2 nanostructures that are prepared with the mole ratio of HAuCl4:CoCl2:TiO2 = 0.015:0.15:1. The SEM image in Figure 3a, b shows that the nanoparticles with an average diameter of about 80 nm are uniformly covered on the tips of TiO2 nanorods, and the morphology of the Co@Au/TiO2 particles looks like fireworks in full bloom. Both dark-field TEM image in Figure 3c and bright-field TEM image in Figure 3d show that most of the nanoparticles attached on tips of TiO2 nanorods are spherical. The high-resolution bright and dark TEM images in Figure 3d, e, f, g, h clearly show that most of the nanoparticles are core-shell nanostructures as indicated by arrows in the figures. Meanwhile, some nanoparticles are well-defined core-shell structures as shown by arrows in Figure 3d, e, while some nanoparticles are complete hollow shell structures as shown by arrows in Figure 3f. In addition, there are many nanoparticles with diameters less than 10 nm adsorbed on the side of nanorods as shown in Figure 3e, f. These different structures of nanoparticles tell us that the replacement process is complex. The Co nanoparticles attached on the tip of nanorods have more opportunities to react with Au3+, and they are replaced more absolutely, and, as a result, the hollow Au shells are formed . However, the Co nanoparticles attached on the middle sites of nanorods have few chances to contact with Au3+ due to space limitation, and they are replaced incompletely, and, as a result, core/shell structures are not formed. In order to identify the bimetallic core-shell structure, the composition and structure of nanoparticles on the surface or tips of TiO2 nanorods are further characterized by high-resolution TEM and the elemental mapping as shown in Figure 3g, h, i. It can be found from Figure 3g that the Co@Au nanoparticles are core/shell structures but they are not uniform. Some ones are well-defined core-shell structures, some are hollow, while some solid nanoparticles have a very thin shell. These different structures of nanoparticles indicate that the replacement process is complex. The local element mapping of this region shows the Co@Au/TiO2 mainly contains Ti, Sn, Pd, Co, and Au. Meanwhile, the nanorods are mainly made of Ti element and small amounts of Sn and Pd elements. The nanoparticle on the tip is composed of Co and Au elements, and small amounts of Sn and Pd elements. In particular, the Co and Au distribution clearly shows the core/shell structure, which is in accordance with the TEM observation in bright-field and dark-field. Figure 3j gives the EDX analysis of this local element mapping region. The content of Ti, Sn, Pd, Co, and Au is 47.39, 0.80, 1.62, 28.55, and 21.53 at%, respectively. On the basis of these characterizations, it can be identified that hierarchical TiO2 nanostructures decorated with core-shell Co@Au nanoparticles have been successfully prepared. The resulting Co@Au/TiO2 also shows a good magnetic response when exposed to an applied external magnetic field as shown by the photograph inset in Figure 3j.
In this paper, we have presented a type of 3D urchin-like hierarchical TiO2 nanostructures decorated with magnetically bimetallic core-shell nanoparticles. The urchin-like TiO2 nanostructures are used as templates, magnetic Co nanoparticles are introduced onto TiO2 nanostructures by electroless plating, and finally, the Au or Ag shell is formed on Co nanoparticles by in situ replacement reaction. The resulting Co@Au/TiO2 and Co@Ag/TiO2 nanostructures not only possess a good magnetic response to an applied external magnetic field but also show enhanced light-absorption ability due to surface plasmon absorption of Au and Ag in the visible region. Decolorization experiments show that the Co@Au/TiO2 and Co@Ag/TiO2 nanostructures can decolorize methyl blue more effectively compared to pure TiO2 nanostructures. The unique structures and enhanced multifunctional characteristics will allow the 3D bimetallic core-shell nanoparticle-decorated TiO2 nanostructures to have potential applications in a wide range of fields.
This work is supported by the National Natural Science Foundation of China (Nos. 11174234 and 51272215) and NPU Foundation for Fundamental Research (No. JC201159).
- Vaneski A, Susha AS, Rodríguez-Fernández J, Berr M, Jäckel F, Feldmann J, et al. Hybrid colloidal heterostructures of anisotropic semiconductor nanocrystals decorated with noble metals: synthesis and function. Adv Funct Mater. 2011;21:1547–56.View ArticleGoogle Scholar
- Banin U, Ben-Shahar Y, Vinokurov K. Hybrid semiconductor–metal nanoparticles: from architecture to function. Chem Mater. 2014;26:97–110.View ArticleGoogle Scholar
- Jiang R, Li B, Fang C, Wang J. Metal/semiconductor hybrid nanostructures for plasmon-enhanced applications. Adv Mater. 2014;26:5274–309.View ArticleGoogle Scholar
- Liu G, Wang LZ, Yang HG, Cheng HM, Lu GQ. Titania-based photocatalysts—crystal growth, doping and heterostructuring. J Mater Chem. 2010;20:831–43.View ArticleGoogle Scholar
- Xiang LQ, Zhao XP, Shang CH, Yin JB. Au or Ag nanoparticle-decorated 3D urchin-like TiO2 nanostructures: synthesis, characterization, and enhanced photocatalytic activity. J Colloid Interface Sci. 2013;403:22–8.View ArticleGoogle Scholar
- Feng LL, Wu XC, Ren LR, Xiang YJ, He WW, Zhang K, et al. Well-controlled synthesis of Au@Pt nanostructures by gold-nanorod-seeded growth. Chem Eur J. 2008;14:9764–71.View ArticleGoogle Scholar
- Levin CS, Hofmann C, Ali TA, Kelly AT, Morosan E, Nordlander P, et al. Magnetic-plasmonic core-shell nanoparticles. J Am Chem Soc. 2009;3:1379–88.Google Scholar
- Chen LY, Fujita T, Ding Y, Chen MW. A three-dimensional gold-decorated nanoporous copper core-shell composite for electrocatalysis and nonenzymatic biosensing. Adv Funct Mater. 2010;20:2279–85.View ArticleGoogle Scholar
- Xuan S, Xiang Y, Wang J, Yu JC, Leung KC. Preparation, characterization, and catalytic activity of core/shell Fe3O4@polyaniline@Au nanocomposites. Langmuir. 2009;25:11835–43.View ArticleGoogle Scholar
- Wang L, Clavero C, Huba Z, Carroll KJ, Carpenter EE, Gu DF, et al. Plasmonics and enhanced magneto-optics in core-shell Co-Ag nanoparticles. Nano Lett. 2011;11:1237–40.View ArticleGoogle Scholar
- Lu Y, Zhao Y, Yu L, Dong L, Shi C, Hu MJ, et al. Hydrophilic Co@Au yolk/shell nanospheres: synthesis, assembly, and application to gene delivery. Adv Mater. 2010;22:1407–11.View ArticleGoogle Scholar
- Xiang LQ, Zhao XP, Yin JB, Fan BL. Well-organized 3D urchin-like hierarchical TiO2 microspheres with high photocatalytic activity. J Mater Sci. 2012;47:1436–45.View ArticleGoogle Scholar
- Yin JB, Zhao XP, Xiang LQ, Xia X, Zhang ZS. Enhanced electrorheology of suspensions containing sea-urchin-like hierarchical Cr-doped titania particles. Soft Matter. 2009;5:4687–97.View ArticleGoogle Scholar
- Guo HX, Zhao XP, Guo HL, Zhao Q. Preparation of porous SiO2/Ni/TiO2 multicoated microspheres responsive to electric and magnetic fields. Langmuir. 2003;19:9799–803.View ArticleGoogle Scholar
- Liang HP, Wan LJ, Bai CL, Jiang L. Gold hollow nanospheres: tunable surface plasmon resonance controlled by interior-cavity sizes. J Phys Chem B. 2005;109:7795–800.View ArticleGoogle Scholar
- Baldrian P, Merhautova V, Gabriel J, Nerud F, Stopka P, Hruby M, et al. Decolorization of synthetic dyes by hydrogen peroxide with heterogeneous catalysis by mixed iron oxides. Appl Catal Environ. 2006;66:258–64.View ArticleGoogle Scholar
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.